Pvc u sheet komadur wa for metal preparation acid pickling tank
PVC‐U KOMADUR FOR METAL PREPARATION PICKLING TANK
INTRODUCTIONTendency of steel material picking up rust when exposed to atmosphere bare. Need ofcleaning presence of oil, grease, rust and black scale on the surface. Mild Steel material isknown for it’s tendency of going under rapid oxidation when exposed to atmosphere bare. Theresult of oxidation is the formation of oxide layer on the surface which we commonly call as‘RUST’. To avoid this oxidation or rusting, the mild steel material is not allowed to get directlyexposed to atmosphere. For this, we generally find rust preventive oil on the surface of mildsteel material. The oil does not allow the material to come in direct contact with air and thusdelays oxidation. However, this doesn’t entirely eliminates the problem of rusting and it onlydelays the process of rust formation.Some mild steel materials are hardened for strengthening and similarly some are weldedduring fabrication. Both these processes leave black scale on the surface.In short, mild steel parts generally have rust and/or grease‐oil and/or black scale on thesurface. All these cause severe problems of bonding if not removed before application of paint.The bare metal being extremely susceptible to atmospheric corrosion should be applied withconversion coating. Before painting, once the rust, oil and scale are cleaned, the bare metal isagain exposed for oxidation. To avoid this, the material has to be coated with some type ofconversion coating which prevents further oxidation before applying paint and also givesadhesion for paint.
PRECLEANING OF MILD STEELDEGREASING ‐ Removal of oil and grease from the surface.Based Degreasing:• Petroleum based solvents have excellent degreasing abilities but are not commonly used because they are highly inflammable.• Alkaline degreasing powders : This is generally a blend of alkalis and surfactants. This is advised to be used under hot conditions. However, alkaline powders are also used under cold conditions as knock out degreasing stage.• Acidic Degreasing : These are solvent based liquids which are acidic in nature. They remove rust as well as grease under cold conditions. The bath of these chemicals is however, much expensive as their concentration is much higher than alkaline degreasing.DERUSTING – Removal of rust and light scale from the surface.These are necessarily acidic chemicals unlike degreasing, which may be alkaline in nature.The chemical is generally a blend of mineral acids like phosphoric acid, sulfuric acid andhydrochloric acid with added inhibitors. Higher acidity will result in faster removal of rust.However, this will affect the life of the coating applied later. Phosphoric acid based derustingchemicals are most suggested for pretreatment of mild steel before applying paint.DESCALING – Removal of heavy scale and heavy rust from the surface. These are strong mineral acid based chemicals with added inhibitors.
COATINGBefore painting, once the rust, oil and scale are cleaned, the bare metal is again exposed foroxidation. To avoid this, the material has to be coated with some type of conversion coatingwhich prevents further oxidation before applying paint and also gives adhesion for paint.The most common types of conversion coating include :∙ Zinc phosphate coating∙ Iron phosphate coatingZinc phosphate coating is crystalline heavy coating gray in colour. While iron phosphatecoating is amorphous conversion coating that ranges in color from iridescent blue to gray.Iron phosphate coating gives minimum sludge formation and hence smoother finish than zincphosphate. Apart from this the bonding characteristics are also good. Iron phosphateprocesses are much easier to operate than zinc phosphate processes and require fewerprocess stages (zinc phosphate coating requires a predip in activation chemical prior tophosphating to have micro crystalline grain structure), but iron phosphates do not provide thedegree of corrosion protection imparted by zinc phosphates.Iron phosphate systems are therefore used for a range of products requiring a durable finishthat are not exposed to severely corrosive environments. Zinc phosphating processes havebeen developed to provide exceptional painted part durability in corrosive requirements.Typical industries using zinc phosphate processes include automotive, appliance and truckand bus.
POST‐TREATMENTAfter a metal surface receives a conversion coating, the surface is water rinsed to remove un ‐reacted conversion coating chemicals and a post‐treatment is applied. The post‐treatment canprovide a two‐ to ten‐fold increase in corrosion resistance and humidity resistance whencompared to conversion coatings without final rinses. Post‐treatments are generally based onchromic acid.Treatment for zinc/iron phosphate include following stages:1. Degreasing : Removal of oil and grease from the surface. This is generally a blend of alkalis and surfactants.2. Water rinse3. Derusting (pickling): Removal of rust and light scale from the surface. These are necessarily acidic chemicals.4. Water rinse5. Activation : This gives more compact and uniform coating of zinc phosphate. This step can be omitted for iron phosphate process.6. Phosphating : This forms coating of zinc phosphate or iron phosphate on the clean surface7. Water rinse8. Passivation : This will seal the pores of phosphating (chromic acid sealing).9. Drying.
PVC‐U KOMADUR WAPVC‐U sheet Komadur WA meets the specific demands for metal preparations industries andelectroplating. PVC‐U sheet Komadur WA is resistance to chemical acid cleaning or picklingusing acids such as HCl, H2SO4, and H3PO4 . Acid pickling is very effective method for removalof rust and mill scale.